HAL Id: hal-02883749
Submitted on 30 Jun 2020
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Alterations of plastics spectra in MIR and the potential
impacts on identification towards recycling
Charles Signoret, Anne-Sophie Caro-Bretelle, José-Marie Lopez-Cuesta,
Patrick Ienny, Perrin Didier
To cite this version:
Charles Signoret, Anne-Sophie Caro-Bretelle, José-Marie Lopez-Cuesta, Patrick Ienny, Perrin
Alterations of plastics spectra in MIR and the potential impacts on identification
Resources, Conservation and Recycling, Elsevier, 2020, 161, pp.104980.
of plastics spectra in MIR and the potential impacts on
ﬁcation towards recycling
a Polymers Composites and Hybrids (PCH), IMT Mines Ales, Ales, France bLMGC, IMT Mines Ales, Univ. Montpellier, CNRS, Ales, France
Keywords: Polymer recycling Sorting MIR WEEE Identiﬁcation Formulated plastics A B S T R A C T
Plastic recycling is mainly limited by their sorting as their natures, forms and formulation are very numerous and most of them are strongly incompatible, leading to poor mechanical properties. Several industrial sorting technologies exist, and others are in development. However, each of them has drawbacks. Especially, NIR-HSI (Near-Infrared Hyperspectral Imagery) is limited by the use of carbon black, mainly as a pigment and UV agent in the case of thermoplastics. MIR-HSI (Mid-Infrared) could be a suitable and viable alternative to resolve this issue. Hence, this work, based on laboratory FTIR-ATR (Fourier-Transform Infrared Attenuated Total Reﬂection), focuses on possible sources of spectral alteration, which could impair identiﬁcation of usual polymers using industrial MIR-HSI. It aims to help simple and rapid laboratory characterization and give tools to avoid mis-identiﬁcation or enable speciﬁc segregation during industrial sorting. First, acquisition parameters were de-graded to simulate those imposed by industrial conditions: short acquisition time, diminished resolution and blank defaults. Then, impact on formulations of usual WEEE (Waste of Electric and Electrical Equipment) plastics were evaluated, with PE, PP, ABS and HIPS as matrices, and carbon black (at diﬀerent concentrations), calcite, talc, titanium oxide and someﬂame retardants as additives. Several patterns found in homemade standard samples were recognized within a stock of about one hundred of real waste samples.
Plastic recycling is viewed as one of the most interesting ways to deal with environmental problems linked to both their production and disposal (Wäger and Hischier, 2015; WRAP, 2008). Nevertheless, reaching interesting properties, as processability, aspect or mechanical performance, is very diﬃcult to achieve as plastics natures, additives, ﬁllers, forms and applications are incredibly diverse. Most of them are non-miscible and even incompatible (Maris et al., 2018), since their blends display functional properties inferior to each of them taken
separately. An eﬃcient and accurate sorting of end-of-life plastics is thus primordial for recycling to be economically pertinent (Vrancken et al., 2017). However, end-of-life management itself also entails ecological impacts. For instance, these plastics needs to be cleaned and thus need water and sometimes detergents. Also, collection and, transport can also bear a severe carbon footprint, especially if these actions are geographically scattered (WRAP, 2008).
Several types of separation technologies exist. They can be classiﬁed in two diﬀerent groups: direct and indirect (Gundupalli et al., 2017). When separation is intrinsically due to property diﬀerences, it is direct.
Abbreviations & acronyms: ABS, Acrylonitrile Butadiene Styrene; APP, Ammonium Polyphosphate; ATR, Attenuated Total Reﬂection; CaCO3, Calcium carbonate or
calcite (chalk); CB, Carbon Black; DSC, Diﬀerential Scanning Calorimetry; FR, Flame Retardant; FTIR, Fourier Transform Infrared; HBCD, Hexabromocyclododecane; HDPE, High Density Polyethylene; HIPS, High Impact Polystyrene; HSI, Hyperspectral Imagery; LIBS or LIPS, Laser Induced Breakdown/Plasma Spectroscopy; LWIR, Long Wavelength Infrared (7.4-14.0 μm or 1350-700 cm−1); MIR, Mid-Infrared (4000-400 cm−1or 2.5-25.0 μm); MWIR, Middle Wavelength Infrared - 2 to 5 μm (5000 to 2000 cm−1); NIR, Near-Infrared – 0,8 to 2,5 μm (12500 to 4000 cm−1); PC, Polycarbonate (from bisphenol A); PE, Polyethylene; PMMA, Polymethylmethacrylate; PP, Polypropylene; PPC or PP copo, Polypropylene copolymer; PPH or PP homo, Polypropylene homopolymer; PVC, Polyvinyl chloride; PS, Polystyrene; RoHS, Regulation of Hazardous Substances; SEM/EDX, Scanning Electron Microscopy / Energy Dispersive X-ray spectroscopy; Sb2O3, Antimony (tri)
oxide; SNR, Signal-to-Noise Ratio; TBBPA, Tetrabromobisphenol A; TGA, Thermogravimetric analysis; THz, Terahertz; WEEE or W3E, Waste of Electrical & Electronic Equipment
E-mail address: email@example.com(D. Perrin).
laboratory scale, precise identiﬁcation and quantiﬁcation of ﬂame re-tardants can be rather burdensome compared to simple infrared spectra, especially with the need of appropriate extraction (Guzzonato et al., 2016a; Otake et al., 2015; Schlummer et al., 2005;
Vilaplana et al., 2008). However, Puype et al. (Puype et al., 2019) re-cently showed that Direct Analysis in Real Time - High Resolution Mass Spectrometry (DART-HRMS) was adequate to rapidly and accurately identify brominated FR at laboratory scale.
Another very common additive, carbon black, which is the most common way to color plastic in black or grey, strongly absorbs in NIR (Beigbeder et al., 2013;Huth-Fehre et al., 1995;Serranti et al., 2012), making NIR-HSI unable to sort dark colored plastics. Its absorption is easily explained by the almost inﬁnite unsaturations conjugation within its graphitic structure (Kang et al., 2016), also explaining its deep black color as it absorbs in the visible range. It also absorbs beyond these boundaries in NIR but also in UV (Allen et al., 1998; Liu and Horrocks, 2002), making it an interesting additive to protect polymeric materials from photodegradation. Consequently, it also impacts Raman spectra more or less depending on the excitation wavelength (Bokobza et al., 2013; Yamaji et al., 2013). More generally, carbon black is used for coloration and UV protection from 0.5 to 2.0 wt. % (Turner, 2018), up to 20 wt. % for electrical conductivity where per-colation is necessary (Probst et al., 2009;Zhou et al., 2006) and up to 50 wt. % for mechanical reinforcement (Kang et al., 2016; Li et al., 2019), especially in elastomers as in tires. As NIR-HSI, the most used technology toﬁnely discriminate plastics according to their natures, is limited with dark plastics, several alternative sorting technologies are subject to extensive research (Grégoire et al., 2011;Huang et al., 2017;
Küter et al., 2018;Langhals et al., 2014;Roh et al., 2017;Wang et al., 2015;Zhao et al., 2018; Zhao et al., 2018). MIR-HSI is one of them (Kassouf et al., 2014;Rozenstein et al., 2017;Signoret et al., 2019a,
2019b). It was chosen in the present study because this technology begins to be commercially available. Also, Fourier-Transform Infrared (FTIR), its laboratory equivalent as it works within the MIR range, was used for a long time for polymer analysis.
The present study aims to complete our previous works on spectral identiﬁcation of polymers through the use of FTIR-ATR (Attenuated Total Reﬂection) with the scope of transposition to MIR-HSI. The ﬁrst study described intrinsic signals of styrenics polymers and their blends (Signoret et al., 2019a). The second one focused on polyoleﬁns and
polymers with close spectra, namely PVC and POM (Signoret et al., 2019b). A third one was about spectral alterations due to ageing of LDPE, PPH, HIPS, ABS and PC in the scope of their identiﬁcation (Signoret et al., 2020). Whereas these previous works focused on characteristic signals of polymers, the subject here is to anticipate how these patterns can evolve because of formulation: carbon black, common mineral ﬁllers and ﬂame retardants. The objective is to de-termine if loaded polymers could still be recognizable, even in degraded acquisition conditions. Also, characteristic patterns related to for-mulation can be useful to quickly identify additives, at least at la-boratory scale, instead of using a heavier technique as ICP (Inductively Coupled Plasma) or X-rayﬂuorescence which can be more time and money consuming. However, accurate quantiﬁcation needs another technique, namely thermogravimetric analysis (TGA).
2. Materials and methods 2.1. Materials
Several polymers were used for formulated standard preparation: ABS reference was Terluran GP22 (Styrolution), HIPS was Polystyrol 485I (Repsol), ABS/PC was Bayblend T85 XF (Covestro), PE was HDPE Alcudia 4810 (Sabic), PP was PPC 83MF10 and PPH 505P (Sabic). Carbon black used in this study was Elftex 570 (Cabot). Several mineral ﬁllers references were also involved: XP12-5630 kaolin (IMERYS), Omya BL calcite (Omya), Luzenac HAR T84 talc (IMERYS) and It is the case with sink-ﬂoat tanks (Gent et al., 2009) where sorting is
based on density diﬀerences. Other examples are froth ﬂotation for surface tension (Wang et al., 2015), trommels for granulometry (Ashkiki et al., 2019), magnetic overhead belts and Eddy current for (para)magnetic properties (Krivtsova et al., 2009). Sorting is indirect when identiﬁcation and separation are performed through two diﬀerent steps (Gundupalli et al., 2017). Generally, these are optical technolo-gies. Items to be sorted are moved on a conveyor belt where a sensor acquires their spectral signature after adequate excitation. Then, these items are physically sorted, usually through the use of compressed air nozzles.
The transposition to industrial dynamical conditions of several static technologies, used at laboratory scale, such as UV-Vis (Gundupalli et al., 2017), NIR (Near-Infrared) (Beigbeder et al., 2013;
Huth-Fehre et al., 1995; Leitner et al., 2003), MIR (Mid-Infrared) (Bae et al., 2019; Becker et al., 2017; Rozenstein et al., 2017), Raman spectroscopies (Bae et al., 2019; Florestan et al., 1994; Roh et al., 2017), LIBS (Laser Induced Breakdown Spectroscopy) (Barbier et al., 2013; Grégoire et al., 2011), X-ray transmission or ﬂuorescence
(Hasan et al., 2011; Mesina et al., 2007) is currently studied. Laboratory analysis generally explores a single sample at a time, on a relatively small spot, can take from several seconds to hours, can be sometimes made with contact to the sample. However, industrial identiﬁcation toward waste sorting is radically diﬀerent. Objects are generally scat-tered along a high-speed conveyor belt and their identiﬁcation must be made remotely within milliseconds to enable sorting at the end of the conveyor. This leads to strong technological diﬀerences, which, with the harsh acquisition conditions, often lead to diﬃcult-to-analyze sig-nals. Available data, spatial and spectral resolutions, signal-to-noise ratio (SNR) can be, at ﬁrst glance, insuﬃcient to enable identiﬁcation. This requires signal processing and use of advanced classiﬁcation al-gorithms (Roh et al., 2017; Spetale et al., 2016; Tachwali et al., 2007;
van den Broek et al., 1998). However, a real physicochemical under-standing of the diﬀerences at the source of classiﬁcation is needed to avoid false identiﬁcations.
Additives and ﬁllers can also have repercussions on sorting. As polyoleﬁns are the main polymers with intrinsic densities below 1 g/ cm3, they can be recovered thanks to tap water sink-ﬂoat. Sadly, an
important fraction is ﬁlled with calcite (calcium carbonate, CaCO3) or
talc (Aluminum Silicate, Al2Si2O5(OH)4) and thus sinks (Maris et al.,
2015). Peeters et al. (Peeters et al., 2014) highlighted density
over-lapping because of the use of ﬂame retardants and styrenic blends, making density separation ineﬃcient. In the frame of WEEE (Waste Electrical and Electronic Equipment) legislation and RoHS (Regulation of Hazardous Substances), numerous widely spread halogenated ﬂame retardants (FR) are now forbidden because of their toxicity. Several other widely used FRs could also become forbidden in the future (Delva et al., 2018; Vilaplana et al., 2008). This imposes sorting ma-terials according to these additives for recycled mama-terials to stay below legal thresholds (Hennebert and Filella, 2018). X-ray transmission and ﬂuorescence are among the most promising technologies towards this goal (Gallen et al., 2014; Kuang et al., 2018; Sharkey et al., 2018). Even in a dual energy conﬁguration, which is well developed and perfectly suitable to metals (Mesina et al., 2007), transmission lacks selectivity between heavy elements. In the case of additive plastics, both con-centration and thickness are unknowns in the Beer-Lambert law whereas concentration was assumed 100% in the case of metals. As it needs to detect way more wavelengths, ﬂuorescence is technologically more challenging and thus more expensive. Solvent extraction of FRs or total dissolution could be very eﬃcient (Grause et al., 2015;
Vilaplana et al., 2009; Zhao et al., 2018), although transposition to industrial scale can be diﬃcult, especially with solvent management. Pyrolysis, towards energy recovery and/or chemical recycling (Ma et al., 2016; Yang et al., 2013) could be seen as the only viable solution, even if rather controlled waste stocks (thus sorted) are needed not to disrupt the process and its eﬃciency too much. Even at
Aeroxide TiO2P 25 titanium dioxide (Evonik). Someﬂame retardants
(FR) were used as received to prepare standard blends: ammonium polyphosphate (APP Exolit AP 423 (Clariant), Dechlorane C25+ (ABCR) and TBBPA reference 330396 from Sigma-Aldrich. Two other FRs were analyzed in powder form because of insuﬃcient available amounts: antimony (tri) oxide (Sb2O3) was Empura (Merck), and HBCD
(1,2,5,6,9,10-hexabromocyclododecane) was the SI-21691 analytical standard provided by Analytical Lab (France). The 112 waste samples were kindly provided by the Suez company from their plants in Feyzin (SUEZ RV DEEE) and Berville-sur-Seine (NORVAL) in France, mainly from WEEE but also from municipal deposits. About two third of them were dark-colored.
2.2. Formulated standards preparation
For ABS, HIPS and ABS/PC transformation, materials were dried at least 16 hours at 80°C before transformation. For large quantity for-mulation campaigns, of the order of kilograms, masterbatches were realized in a Rheomix 3000 internal mixer (Haake). Masterbatches were then diluted with a Clextral 900 BC21 twin screw extruder (Clextral). For small quantity formulation campaigns, of the order of tens to a hundred grams, a DSM MC40 microextruder (Xplore) was used. Masterbatches were made then diluted twice to four times depending on the desired concentration. The minimum of two-step was chosen to ensure concentration homogeneity as ﬁrst mixes are often hetero-geneous, especially in internal mixer. All materials were processed between 210 and230°C. For spectral characterization, especially in FTIR-ATR, standard samples were produced in the form of disks with 25 mm diameter and 1.5 mm thickness. A Zamak-Mercator injection molding machine was used in this purpose.
2.3. Thermogravimetric analysis
A Pyris 1 TGA provided by Perkin-Elmer was used to estimate carbon black loadings within real waste samples and produced stan-dards. Temperature was raised from 30°C to 900°C at 10°C/min. Samples were analyzed under nitrogen at 20 mL/min up to 650°C, where most of polymeric parts are degraded, then under air at same ﬂow where carbon black degrades. At least, three measures were averaged for each batch. Curve examples are given inappendix A. It can be seen that virgin samples are not totally degraded before after the gas switch. Thus, the≈1.8 wt. % loss attributed to ABS must be subtracted from the carbon black rate. Additionally, theﬁnal mass is subjected to tare imprecision and losses below 200°C can be associated to volatiles, especially humidity. Thus, the carbon black loading rateτNC(wt. %) is
calculated as follows from mass lossesΔm(ΔT)X(wt. %) whereΔT (°C)
corresponds to temperature ranges and X refers to samples or refer-ences: = − − − ∘ − × − − ∘ ∘ ∘ ∘ τ m C m C Δ (650 900 ) Δ (200 900 ) NC sample m C m C m C sample Δ (650 900 ) Δ (200 650 ) Δ (200 900 ) ref sample ref 2.4. FTIR Spectroscopy
A Vertex 70 FT MIR spectrometer from Bruker with an ATR unit equipped with a diamond crystal was used. Unless indicated otherwise, resolution was at 4 cm−1, 16 scans for background acquisition and 16 scans for the sample spectrum. Most of the samples were directly ana-lyzed on the crystal. Some were cut to obtain better acquisition as ATR is sensitive to surface aspects. Analyzed surfaces were cleaned with ethanol and left to dry. Spectra were acquired from 4000 to 400 cm−1 and analyzed thanks to the OPUS software provided with the spectro-meter. Matlab 2018 and Origin 9 were also used for further processing. FTIR-ATR (Attenuated Total Reﬂection) was chosen for convenience and to be closer to HSI cameras as both are reﬂective technologies. For carbon black powder analysis, a transmission unit was used on KBr (potassium bromide) disks at a 4 cm−1resolution, 32 scans for back-ground and for sample.
2.5. SEM/EDX: Scanning electron microscopy– Energy dispersive X-ray spectroscopy
SEM analysis was performed with a Quanta 200 FEG from Thermo Fischer Scientiﬁc on waste samples. The use of an Oxford energy-dis-persive X-ray spectroscopy (EDX) sensor allowed to carry out elemental imaging of samples.
2.6. Spectra comparison methodology description
The overall methodology of this work is based on the use of charts as
Table 1. It gathers every encountered within 10 cm−1wide columns. Other charts are available in supporting information, covering both MWIR and LWIR, and every polymer described in previous works. The applied colors relate the visually relative intensities of the corre-sponding signal within the considered range, similarly with the“strong” or“weak” mentions frequently found in correlation tables. Purple, red, orange, yellow and light yellow respectively correspond to “very strong”, “strong”, “medium” “weak” and “very weak”. Blue is used for signals highly variable in intensity. These charts are useful as signals and speciﬁc patterns of a chemical species or a family are highlighted by columns empty elsewhere. Also, they can be used in the other way when looking for an unknown encountered peak. However, one should pay attention to complementary signals, as an isolated peak can cor-respond to several species.
3. Results and discussion 3.1. Degraded acquisition
3.1.1. Background/blank default: Atmospheric IR absorbent species - CO2
CO2and H2O are more and more visible as background/blank is too
old compared to current acquisition and as intrinsic signals from the polymer are weak as seen onFig. 1. As all analyzed surfaces wereﬁrst cleaned with ethanol and left to dry, observed water signals are prob-ably corresponding to atmospheric water. The polymer corresponding to this spectrum can still be identiﬁed as calcite loaded PVC. Calcite speciﬁc signals are described in Part 3.3. PVC is mainly identiﬁed through its 700 and 610 cm−1pattern characteristic of C-Cl stretching (Signoret et al., 2019b). H2O signals, seen from 4000 to 3500 cm−1for
MWIR, and 1900 to 1300 in MIR, framed in blue onFig. 1, could be perceived as noise but its particular pattern is characteristic of several gaseous species, preventing confusion with plastics. Whereas rotational levels are strained in condensed phases by surrounding molecules, they are“pure” in gas phase, each gap between observed lines corresponding to a distinct excitation level, explaining their regularity and respective heights (Hollas, 2004). Other atmospheric species as nitrogen or oxygen cannot absorb in infrared as asymmetry cannot be introduced in their dipole moment with bending (Hollas, 2004). However, they can in Raman as excitation mode is diﬀerent (Fletcher and Rayside, 1974) and this could strongly disrupt industrial applications.
Way more pronounced than H2O, CO2has two very famous bands at
2370 and 2340 cm−1 in MWIR. Excluding isocyanate (N=C=O) stretching at 2270 cm−1which can be residually found in some poly-urethanes, and nitrile (C^N) stretching at 2237 cm−1for ABS or SAN,
no speciﬁc polymer signals were found from 2000 to 2500 cm−1
(MWIR chart in supporting information). Thus, this signal should not mask important peaks. In LWIR, CO2has a very thin peak at 670 cm−1
(Hossain et al., 2014). Within 10 cm−1, as seen in the LWIR chart in supporting information, calcite, TBBPA and Dechlorane have a peak here, but being larger for theﬁrst one, and accompanied by many other peaks for the two others, as described further below. Checking com-plementary signals rapidly eliminates any doubt.
Atmospheric species should moderately impact polymer industrial identiﬁcation as concerned ranges do not overlap each other or signal nature is diﬀerent (as with atmospheric water). It is thus important to consider them separately in a classiﬁer learning phase, not to include atmospheric parameters in plastic identiﬁcation, as they can be hardly controllable at reasonable costs. Also, they can represent a numerical
“dead weight”, inducing useless data treatment.
3.1.2. Short acquisition time: diminishing number of scans in FTIR
Figure 2.a) shows the spectral evolution by diminishing the number of scans in FTIR-ATR on an ABS standard. Both sensor noise and “at-mospheric noise” are ampliﬁed with reduction of scans. In this parti-cular case, it does not challenge identiﬁcation as the polymer signal was strong. In industrial conditions, acquisition time is very short for ma-terial throughput reasons but several pixels are acquired for each ob-ject, mimicking plural scans. It can however be expected that Signal-to-Noise Ratios (SNR) should be far lower.
3.1.3. Evolution with resolution
Figure 2.b) shows the impact of resolution reﬁnement on a PP re-ference MIR spectrum. A strongly deﬁned spectrum tends to display stronger noise, especially here, where only one scan was performed for each spectrum. Again, atmospheric species are fostered. Thus, resolu-tion and acquisiresolu-tion time must be tuned altogether. With degraded resolution, peaks get convoluted and weaker, as they tend to be par-tially averaged with baseline. Especially here, the four distinct peaks of PP (C-H stretching) between 2800 and 3000 cm−1merge into a single shape (blue frame inFig. 2.b)). It happens even more rapidly with CH3
C-H bending at 1375 cm−1(purple frame and magniﬁcation) where the presence of shoulder underlines crystallinity (Signoret et al., 2019b). It is evident that convolution intervene faster as peaks are close and weak. Noise can appear milder at 4 cm−1resolution than on its equivalent on
Fig. 2.a) but it is probably mainly due to scaling and numerical oﬀsets diﬀerent which were diﬀerently chosen here to highlight convolution of signals. Finally, the black framed magniﬁcation ofFig. 2.b) shows how a weak signal disappears as it is averaged with the baseline. It is the example of the 2725 cm−1peak, very speciﬁc to PP as it is alone within its column in the MWIR chart (supporting information). Combined with rather weak signals due to short acquisition time, this can lead to im-portant information loss, detrimental to fast identiﬁcation.
3.1.4. Conclusions on degraded acquisition
Atmospheric species can display important signals but are located in speciﬁc zones and should not negatively impact polymer identiﬁcation if well taken in account. Short acquisition time mainly impacts signal-to-noise ratio whose degradation can be tempered with radiation source intensity. However, this can lead to serious heating. The depreciation of resolution leads to the convolution of peaks and global reduction of intensities, which can lead to the visual disappearance of small peaks.
Figure 1. Pathologic FTIR-ATR spectrum of waste sample n°1.37 & corresponding background spectrum - signals of CO2framed in red, H2O in blue, PVC in green and
3.2. Carbon black impact on MIR spectra
As carbon black strongly absorbs in UV, in the visible range and in NIR, one could worry about its absorption in MIR and possible induced disturbances in polymer identiﬁcation. In the purpose to qualify this impact, carbon black powder and homemade dark colored samples were characterized in FTIR-ATR.
3.2.1. Carbon black-KBr disks in FTIR-Transmission
To avoid spectral defects from ATR, which distorts baselines as in-frared penetration depends on its wavenumber, carbon black was analyzed in transmission after dilutions within dried KBr.Fig. 3shows spectra obtained with 1.00 and 0.25 wt. % disks which were equally totally black to the naked eye. At 1.00 wt. %, transmission is at 0% on the whole range and the absorbance curve highlights the sensor's limit of sensitivity. At 0.25 wt. %, transmission is below 2% on most of the
Figure 2. Impacts of acquisition parameters in FTIR-ATR on the quality of spectra: a) Number of scans reduction on an ABS standard with a 4 cm−1resolution b) Resolution degradation on a PP standard with 1 scan per measure– blue frame for C-H stretching convoluting signals and purple for crystallinity marker
range and rapidly rises up to 20% on the last 1000 cm−1. Logically, absorbance slightly and steadily decreases from 2000 to 400 cm−1, from 2 to 1 A.U. It appears that a higher carbon black content leads to a higher absorbance baseline (and lower transmission baseline).
No special features, as C-H, O-H or C=O marks, can be observed, meaning that the graphitic structure is rather predominant and material is not visibly oxidized. As the graphitic sheets are semi-inﬁnite and thus double bonds highly conjugated, absorption seems continuous from UV up to MIR.
3.2.2. 2 wt. % loaded PE, PP, HIPS & ABS samples
PE, PP, HIPS and ABS spectroscopic standards were made and controlled by TGA at 2 wt. % carbon black. This concentration was chosen as it is the most current loading rate for coloring thermoplastics and for protecting them from photodegradation. As speciﬁed pre-viously, higher rates are applied for elastomers reinforcement, or electrical conductivity, which are both scarce among WEEE.Fig. 4was produced without numerical oﬀsets of the curves and by repeating each measure four times on diﬀerent specimens or spots. The resolution was 4 cm−1and acquisition was made in 16 scans. Same parameters are applied for all data given from this point. The most important feature is a shift of absorbance baseline, more or less important depending on the polymer, but generally of about 0.01 to 0.02 A.U. It is coherent with spectra of carbon black alone in KBr, as it is a continuous absorption. Interestingly enough, HIPS and ABS baselines were already above 0 U.A., at about 0.04 U.A. at 4000 cm−1and at about 0.07 U.A. at 400 cm−1, highlighting the ATR defect. This defect, intrinsic to ATR, fosters stronger absorption at lower wavenumbers because infrared penetra-tion within the sample depends on its wavenumber. This defect is also more or less intense depending on the quality of acquisition, mainly due to the surface-crystal contact.
Even though carbon black intrinsically absorbs less at low wave-numbers, its presence seems to amplify this defect as the shift is of only 0.01 U.A. on the left side and up to 0.06 U.A. on the right side. This can be explained as infrared rays penetration is aﬀected by the presence of carbon black. Eﬀects on polymer peaks intensity seem negligible in this concentration range. Identiﬁcation through MIR seems unaﬀected for these polymers at these loading rates.
3.2.3. ABS at diﬀerent carbon black loading rates between 0.05 & 4.50 wt. %
To study further the impact of carbon black on MIR spectral fea-tures, several ABS standards were made at diﬀerent loading rates of carbon black. Always under TGA control, aﬁrst series from 0.5 to 2.0 wt. % was made in extrusion from a≈20 wt. % masterbatch made using an internal mixer and aﬁrst dilution which was checked at 4.5 wt. %. A second series was made from the 0.5 wt. % batch in a mi-crocompounder to reach loadings from 0.05 to 0.20 wt. %.Appendix B
shows pictures and spectra of spectroscopic standards made from these batches, 5 spectra by sample and no normalization or numerical oﬀset. Even at 0.05 wt. %, the obtained sample was totally black to the naked eye, visually diﬃcult to diﬀerentiate from other samples. Grey material was obtained from purging the apparatus but carbon black was not detectable through TGA. Baseline shift and distortion through ATR defect steadily follows the carbon black rate. ABS characteristic peaks heights do not seem to evolve. The concentrations between 0.05 and 0.20 wt%, in light pink display very close spectra. The magniﬁcation on 2100 to 2000 cm−1shows that the baseline progressive shift is still observable even though in the same order of magnitude than repeat-ability.
To quantify previously described phenomena,Fig. 5shows integral values obtained from the spectra in order to quantify the observed baseline shift and intrinsic signals intensity. Fig. 5a) shows signals chosen to evaluate these phenomena: C-H stretching from 3100 to 2800 cm−1, both aliphatic and aromatic; C^N stretching from 2255 to 2220 cm−1; aromatic C-H bending from 800 to 720 cm−1. Area between spectrum and a straight line drawn at the base of each peak were considered in this case. No normalization but repeatability was applied as the whole range should be impacted by eﬀects to qualify. As no peak should be spared, none can serve as a reference for normalization. A baseline indicator was chosen by integration between spectra and the X axis on the 2100 to2000 cm−1range. This choice was made because this range is free of signals attributed ABS, degraded ABS (Signoret et al., 2020) or other parasites as moisture. Also, integration averages the impact of individual values on this range, thus attenuating noise perturbation. Finally, this range was little aﬀected by ATR de-formation.
Fig. 5 b) shows that results dispersion is important on speciﬁc
polymer signals and hampers a clear discussion. However, C^N and C-H stretching signals seem to slightly decrease with also a reduction in
dispersion. Polymer lesser absorption could be explained as it receives less incident signal because of carbon black and as its reﬂected signal gets also partially absorbed. Aromatic C-H does not show a decrease and could even exhibit a reduction in dispersion toward higher values. These contradictory trends can be explained by the previously observed ATR deformation, fostered by carbon black, which promotes absorption at low wavenumber. Potential eﬀects of pi-stacking between carbon black and aromatic cycles of ABS seem unlikely as this pigment stays under an agregated form, thus not very well dispersed. It is also partly oxidized and does not exhibit a highly organized structure. Purer, better dispersed and better structured forms of mineral carbon, as nanotubes, graphite or graphine could however exhibit pi-stacking interactions.
Fig. 5 c) displays the chosen baseline indicator evolution with carbon black concentration, which proves to be rather linear on the considered scope, respecting the Beer-Lambert law. Last points at 4.5 wt. % tend to be above the regression, probably because of the ATR eﬀect. Despite the important values dispersion, the correlation factor is rather satisfactory (R²=0.986). The 1.98 intercept value is coherent to the values of virgin samples. Low loading samples do not seem to align perfectly as seen on the magniﬁcation. Concentrations were too low to be conﬁrmed by TGA. As they were made diﬀerently, diﬀerences in dilutions with other samples could explain this. It should be emphasized that diﬀerences of polymer nature, chosen shape, especially surface aspect and acquisition quality strongly disturb these correlations. Here, data were wellﬁtted because all above-mentioned parameters are al-most identical even though results are pretty dispersed.
3.2.4. Real waste samples
Thirty-seven black colored samples among the stock were analyzed using TGA. Seven had undetectable carbon black levels (below 0.1 as otherﬁllers were also considered here). Twenty-one had concentrations between 0.5 and 2.0 wt. %. Six others had concentrations up to 4 wt. %.
Two PVC samples showed 8 and 18 wt. % which could be caused by other additives as PVC is often heavily formulated. Identiﬁcation through FTIR-ATR was not challenged. Baselines and peak heights were more inﬂuenced by surface aspect and acquisition than measured carbon black concentrations. Indeed, ATR is very sensible to the contact quality between the sample and the ATR crystal, a default which does not transpose to HSI as measure is done remotely. However, other sources of acquisition degradation could be expected, as spatial non-uniformity of infrared irradiance, or sensibility to surfaces orientation and objects heights.
As an exception, one PP sample, whose spectrum is shown onFig. 6, presented a carbon black loading rate evaluated around 25 wt. % in TGA. The ﬁrst ABS masterbatch, measured at 21 ± 2 wt. %, is also plotted for comparison. However, because the high carbon black con-tent prevented disk injection for rheological reasons, test bars were injected instead. This waste sample had the mention“Velostat” which is described as conductive polymer (Mazaheri et al., 2009). This is con-sistent with the high carbon black loading measured. Its spectrum baseline is strongly slanted (ATR defect), going from 0.03 to 0.08 A.U., showing a strong absorption from carbon black, whereas intrinsic sig-nals amplitude is below 0.02 A.U. Also, the bottom of the peaks is strangely slanted. This could be explained by a deﬁcient response of Fourier Transform to phase shift (Keeler, 2004;Ledford et al., 1980). The spectrum is however visually recognizable as PP, with four peaks for aliphatic C-H stretching from 2840 to 2950 and two peaks at 1450 and 1375 cm−1respectively for C-H bending of CH2and CH3. The 21
wt. % ABS reference however is hardly recognizable as its signals are generally weaker than PP on the whole MIR range through ATR (Signoret et al., 2019b). Only the strongest signals, aromatic C-H de-formation at 760 and 700 cm−1, are clearly visible whereas others seem only baseline defects. This hints that only the strongest signals will survive. Interestingly enough, even on such a distorted spectrum, peaks
Figure 4. MIR spectra of virgin (red curves) and 2 wt. % carbon black loaded (black curves) polymer standards– PE, PP, HIPS & ABS – 4 spectra by sample, no normalization or numerical oﬀset
Figure 5. a) Integration zones on ABS FTIR-ATR spectra– green, pink and blue for b), grey for c); b) Intrinsic peaks integrations evolution with carbon black loading rates; c) Baseline“height” evolution with carbon black loading rates – no normalization, 5 measures/batch, 4 cm−1resolution and 16 scans by acquisition
Figure 6. MIR comparison of sample n°1.46 (exception within waste stock) to ABS standards at 4.5 and≈21 wt. % carbon black – sample identiﬁed as PP loaded with≈25 wt. % carbon black – no normalization, baseline correction or numerical oﬀset – black frames for PP peaks, red for ABS
Figure 7. MIR spectra of common mineralﬁllers – kaolin (green), calcite (black), talc (blue), titanium oxide (red) – wavenumbers in corresponding colors
retain their exact wavenumber. Finally, baselines for 4.5 and 21 wt. % overlap for the highest wavenumbers whereas the 21 wt. % spectrum should be far above, closer to the waste sample as they share close concentration. This indicates that acquisition was not optimal for the heavy loaded sample, adding to the poor visibility of characteristic signals. If signal is still suﬃcient in industrial conditions for such loadings, strong correction of baseline could be applied to make the spectrum exploitable despite the loss of information.
3.2.5. Conclusions on carbon black impact on MIR spectra
Because of its chemical nature, carbon black strongly absorbs from UV to NIR, even at low loadings as 0.5 wt. %, conferring its color, its protecting ability toward polymers and the current diﬃculty to sort most of dark plastics in an economical way. It displays a continuous absorption in MIR, but in a way less dire manner, especially for the lowest wavenumbers. For concentrations typically applied for colora-tion / proteccolora-tion purposes, between 0.5 and 2.0 wt. %, identiﬁcacolora-tion is not impacted for FTIR-ATR. Similar results could be expected that MIR-HSI is also whereas NIR-MIR-HSI is generally reported ineﬀective (Beigbeder et al., 2013; Huth-Fehre et al., 1995; Serranti et al., 2012). The main noticed eﬀect of carbon black in FTIR-ATR is a shift of the baseline toward higher absorbance, proportional to concentration, ac-cording to the Beer-Lambert law. The ATR distortion of baseline is also promoted. Higher loadings (> 20 wt. %) corresponding to very speciﬁc conductive applications in thermoplastics and mechanical reinforce-ment in elastomers are disruptive toward identiﬁcation which is still possible depending on the material. However, as infusible materials, elastomers should be industrially segregated as unsuitable to mechan-ical recycling. Thus, highly distorted spectra, which hint for high carbon black concentration, should lead to refusal.
3.3. Usual mineral ﬁllers 3.3.1. Powder references
Calcite and talc are widely used as ﬁllers, to reduce costs mainly for the former, but they also bring stiﬀness for the latter and unfortunately
density for both (Maris et al., 2015). Titanium oxide (TiO2) is widely
used as an opaciﬁer and a whitening agent. With kaolin, these three additives were analyzed in FTIR-ATR, directly in powder form (Fig. 7). They display very few and very weak signals in the MWIR range, even none for TiO2, leaving their lines almost empty in the corresponding
chart in supporting information. However, corresponding wavenumbers are in usually empty ranges: three sharp signals between 3620 and 3695 cm−1 for kaolin; a bump at 2510 cm−1 for calcite; three signals at 3675, 3555 and 3415 cm−1 for talc. In the LWIR range, they display
very strong, very large (except for kaolin) and distinctive signals: for kaolin a very characteristic quadruplet 1114, 1032, 1008 and 914 cm−1, and three signals between 430 and 540 cm−1 (oﬀ range); for calcite a very broad asymmetric signal at 1406 cm−1 and a very speciﬁc
signal at 874 cm−1; for talc a very broad signal at 1010 cm−1, a very
speciﬁc signal at 670 cm−1 and three intense signals between 465 and 425 cm−1 (oﬀ range); for TiO
2 a wide and strong signal from 800 to 500
cm−1, at the limit of LWIR. It is interesting to note that the 670 cm−1 signal for talc and the 873 cm−1 for calcite are in rather empty columns
within the LWIR chart (supporting information), thus enabling rapid identiﬁcation. However, conﬁrmation should be done with the large and intense signals.
3.3.2. Real waste samples
Because of the speciﬁcity of these wavenumbers (totally or almost alone in their columns of the charts in supporting information), even weak signals could be easily seen on numerous plastic waste samples, every encountered PVC and most of polyoleﬁns samples. On the dis-played example of polymer waste in Fig. 8.a) and b), both calcite and talc can be very clearly seen in LWIR, especially with the speciﬁcity of respectively the 873 and the 670 cm−1 peaks, which enabled rapid
identiﬁcation for most of the waste stock. Impressively enough, the ﬁllers very weak peaks in MWIR are also visible on part a). The 37 dark plastic waste samples analyzed above in TGA for their carbon black concentrations were also studied in SEM/EDX for other additives. Most of the polyoleﬁns contained talc and/or calcite and spectroscopic marks described here were observed each time. Residual weights in TGA
indicates that typical loading rates were between 10 and 20 wt.% which is coherent with industrial use. Only 3 styrenics were found to contain ﬁllers according to EDX and characteristic peaks were visible on the spectrum of only one of them.
The signal from 800 to 450 cm−1of TiO2was indicated in orange in
the charts because it was less visible within real samples as its loading rates were probably weaker as it is a pigment rather than a ﬁller. Indeed, spectral marks of TiO2were formally conﬁrmed on only one
sample (Fig. 8.c)), particularly white, of the hundred available ones even if SEM-EDX revealed traces in 6 of the 37 analyzed samples. Its main signature is conﬁned between 500 and 600 cm−1 and is
re-presented by a round band. The other weak round peak at roughly 1440 cm−1overlaps with CH2deformation and is thus masked in numerous
polymers (as polyoleﬁns, styrenics or polyamides). Use of other ad-ditives, especially talc, and bad acquisition leading to strong ATR baseline defect often lead to doubts about signals which could indicate TiO2presence. In HSI application, almost no signals are speciﬁc, except
for a rise on the lowest wavenumbers in LWIR. No sample was found with kaolin peaks, in accordance with the current limited commercial use of thisﬁller. If present in suﬃcient amount, it could be detected through its peaks between 3693 and 3620 cm−1since peaks of talc between 3675 and 3415 cm−1were visible despite their low intensity. Also, its speciﬁc peaks at 1115 and 540 cm−1should enable
identiﬁ-cation, even in presence of talc or calcite that could overlay its signals.
3.3.3. Conclusions on usual mineralﬁllers
In general, talc and calcite were the main additives to display visible marks on the real waste samples spectra among the studied stock. It can be assumed that other additives are in too low concentration or do not
exhibit important enough infrared signature. Interestingly enough, after sink-ﬂoat separation, most ﬂoating polyoleﬁns still displayed peaks characteristic of aﬁller, even if weaker than in sinking ones. Combined with TGA or calcination, FTIR-ATR can rapidly give natures and con-centrations ofﬁllers, instead of more laborious methods as ICP or X-rays ﬂuorescence. Described ﬁllers can be seen in MWIR even though their speciﬁc signals are very weak and diminished acquisition parameters will surely make them undetectable. Consequently, polymer identi ﬁ-cation should not be disrupted in MWIR. It is not the case in LWIR because of their large signals, which can partially mask speciﬁc signals of polymers. It is thus important to identify and take into account their patterns when building classiﬁcation algorithms. By considering these signals as those ofﬁllers, it could then facilitate the matrix identiﬁca-tion. Filler detection could also be a segregation tool, as it would be devoted mainly to polyoleﬁns and PVC. Finally, it could be interesting to check additives eﬀects on NIR. If impacts are important on identi-ﬁcation, it could render MIR more interesting, even in the case of light-colored plastic waste. However, a real comparison of the two technol-ogies in such waste stocks should be pertinent at least at pilot scale.
3.4. Flame retardants
3.4.1. Powder and polymer references
Flame retarded polymers are widely used in electronic and electrical equipment and furniture as they can be subjected to ﬁre hazards. However, many ﬂame retardants (FRs) which were popular a few decades ago because of their performance at low loadings are now progressively forbidden, or at least greatly depreciated in reason of their health and environmental hazards, especially halogenated FRs
Figure 8. MIR spectra of a waste samples containing spectrally visibleﬁllers – a) & b) A sample with both talc (blue frames) and calcite (orange frames) visible, from 4000 to 2400 and from 2100 to 400 cm−1– c) A sample with visible titanium dioxide (green frame)
LWIR but could disrupt the matrix identiﬁcation as it complicates the spectrum. It is however probably undetectable in MWIR.
In MWIR, TBBPA is rather subtle and was mainly seen for rather high loading (34 wt. %) through its 3475 cm−1peak (Liu et al., 2016), as seen squared in blue on the left part ofFig. 9.c). As well, its numerous LWIR signals are hardly visible below 17 wt. %. The 1173 cm−1is probably the most visible marker. For ABS and ABS-PC, the 730 cm−1is also pretty remarkable as it inserts itself just between the two aromatic C-H peaks. However, it is not visible in HIPS as the higher peak is lower (750 instead of 760 cm−1) and larger, covering it. Outside of ranges covered by MWIR and LWIR, the peak at 1471 cm−1is also very visible in styrenics as it inserts between the ones at 1493 and 1452 cm−1. Just above, a small but sharp peak can be seen at 1555 cm−1 only for highest loadings. Finally, a large band at 1739 cm−1 is visible for higher loading but could be mistaken for polymer ageing carbonyls.
Spectra ofﬂame retardants above, with the addition of HBCD and Sb2O3are given inappendix Cfor better readability.
3.4.2. Real waste samples
Very few samples within the studied waste stock presented re-markable spectroscopic patterns ofﬂame retardants. Accordingly, only one of the thirty-seven samples studied in SEM/EDX showed presence of ﬂame retardant, a brominated one in this case. Except with PVC, most of marked foreign signals were associated to calcite, talc and/or ageing. PVC often displays a peak at 1730 cm−1associated to phthalate plasticizer and/or stearate thermal stabilizers (Signoret et al., 2019b). This can be explained as the waste stock was not primarily chosen to studyﬂame retardants and probably went through X-ray sorting.Fig. 10
shows two waste samples which were identiﬁed as containing ﬂame retardants. The n°5.11 was identiﬁed as HIPS and several Dechlorane peaks were observed, especially at 1470, 1282, 592 cm−1and between 1168 and 831 cm−1. The peak at 763 cm−1is hinted through a subtle shoulder of the 750 cm−1peak of HIPS. Sample n°5.30 was identiﬁed as TBBPA loaded ABS, with especially the double peaks of 1272 + 1238 cm−1, the one at 1555 and the one at 867 cm−1. The 730 cm−1peak is also well visible between the styrene peaks and the 1471 cm−1is seen as a shoulder. Fig. 10 highlights that both Dechlorane and TBBPA creates“interstitial” peaks within styrenics, between the 1452 and 1493 cm−1peaks (outside of LWIR) and between 750+695 (PS) / 760+700 (SAN) (at the limit of LWIR). However, they are not very intense and pretty close from other peaks. Depreciated resolution and sensibility can be fatal to their detection.
3.4.3. Conclusions onﬂame retardants
It appears that Dechlorane and APP are well visible in LWIR (from 8 wt. % and 16 wt. % loadings respectively), especially with signiﬁcant and numerous signals (Dechlorane) or broader signals (APP). TBBPA is harder to identify unless a high loading (34 wt. % here) is applied. APP also strongly distorts MWIR spectra with a large baseline elevation from 2600 to 3400 cm−1, which could be mistaken with acids but a bump at 3165 cm−1is speciﬁc. Dechlorane is impossible to detect in MWIR and TBBPA O-H stretching can be spotted at 3475 cm−1, but only for higher loadings.
Flame retardants industrial detection in MIR seems diﬃcult as sig-nals are subtle, except for APP which could disrupt polymer recognition as its bands could mask the characteristic polymer spectra. Further studies on a larger scope ofﬂame retardants (especially PBDE, poly-bromodiphenylethers) and a waste stock rich inﬂame retarded plastics could ensure their detection and pseudo-quantiﬁcation in FTIR without relying on heavier techniques as XRF. Hyperspectral detection seems compromised and industrial segregation of halogenated plastics should be done thanks to a more reliable technology as industrial XRT or XRF. However, this also means that polymer identiﬁcation in MIR-HSI is unlikely to be hindered byﬂame retardants presence.
(Aldrian et al., 2015; Peeters et al., 2014; Schlummer et al., 2005;
Stenvall et al., 2013). It is thus interesting to detect these now forbidden or phased out FRs within waste plastics. Elemental techniques as X-ray transmission or ﬂuorescence, or LIBS, are rather performant. However, mainly X-ray transmission is nowadays applied in industrial and eco-nomic conditions. Unfortunately, this technology is limited towards distinction between elements heavier than oxygen within polymeric matrices.
Because of their eﬃciency at low loadings, brominated ﬂame re-tardants were quite popular and can be found from a few percent to about 15 wt. % within plastic waste (Guzzonato et al., 2016b;
Schlummer et al., 2005). Tetrabromobisphenol A (TBBPA) and Hex-abromocyclododecane (HBCD) are amongst its main representatives (Puype et al., 2019). Antimony trioxide (Sb2O3) is also often used in
synergy with these FRs. As only TBBPA was available in suﬃcient quantities to product plastic samples, HBCD and Sb2O3 were only
stu-died as powders. Less frequent, chlorine based FRs as dechlorane are also found (Schlummer et al., 2005). Because of the ban of some ha-logenated FR, phosphor based FRs as ammonium polyphosphate (APP) are getting more and more popular (Peeters et al., 2014). FRs speciﬁ-cally cited above were chosen to produce standard samples because of their common use within plastics and because they were rapidly available for experiments.
As seen on Fig. 9.a), ammonium polyphosphate (APP) displays a very wide signal from 2700 to 3300 cm−1. It covers almost all the
MWIR range as seen in the associated chart in supporting information. Three mounts culminate at 2885, 3015 and 3165 cm−1, associated to
the O-H bounds of the phosphate groups. The one associated to the highest wavenumber is particularly visible on formulated samples. For styrenics, this large band tends to mask polymer characteristic signals, potentially challenging identiﬁcation. APP displays numerous, rather strong signals and broad signals (50 to 100 cm−1 wide) in the LWIR
area. The 1246 cm−1 stands out but the 4 peaks from 1080 to 798 cm−1
oﬀer a very distinctive pattern. The three peaks below 550 cm−1, thus
out of the LWIR range, are reminiscent of talc but at higher wavelength and more spaced out. The 1425 cm−1 peak, above LWIR, tends to add
up to the very common 1450 to 1470 cm−1 peak associated to CH 2
deformation. The 1680 cm−1 is too weak and present in an area often
disturbed by carbonyl species produced by ageing. Overall, by its nu-merous and large signals, APP can complicate identiﬁcation as it be-comes the main component of the spectrum in the MWIR and LWIR ranges. Interestingly enough, the 1375 cm−1 and 760 to 750 + 700 to
695 cm−1 peaks, respectively characteristic of PP and styrenics ﬁll the
gaps between APP peaks. It would be also the case with the 730 to 720 cm−1 signal of PE. In the range between MWIR and LWIR, roughly from 2000 to 1400 cm−1, APP does not disturb identiﬁcation, which is
mainly based on the carbonyl peak (Signoret et al., 2020) (as PC, PMMA, PET and PA).
Dechlorane C25+ (Fig. 9.b)), a chlorinated FR, displays rather weak C-H stretching signals at 2950, 2910 and 2850 cm−1, typical of
ali-phatic C-H stretching, in accordance to its chemical nature. These wa-venumbers are already covered by most polymers. This additive seems thus practically impossible to detect in MWIR. However, in LWIR, it possesses very numerous, strong and sharp signals. The 1282 cm−1 is
characteristic as it is in an empty column in the LWIR chart. The several peaks, from 1168 to 831 cm−1, covers a more occupied area as none of
them are in empty column and they tend to make the obtained pattern way more complex. The six peaks from 763 to 592 cm−1 possibly
correspond to C-Cl stretching as there are 12 chlorine atoms within the structure which can vibrate with multiple symmetrical and asymme-trical modes. With almost equal heights of four of them and equal wavenumbers gaps between the ﬁrst three, they create a very dis-tinctive pattern. Also, they modify the general look of the characteristic aromatic C-H deformation of styrenics, two peaks from 760 to 750 cm−1 and from 700 to695 cm−1. Especially, a new sharp peak appears just between them. As APP, Dechlorane should be easily detected in
3.5. Complex samples examples
Several “complex” samples were found among the plastic waste stock, in the sense that they correspond to several materials bonded
together and could negatively aﬀect sorting operations. Fig. 11.a) shows a few examples. The top one (n°1.9) corresponds to an ABS square, characterized by the acrylonitrile peak at 2237 cm−1framed in green, in which was included an elastomeric cylinder. This part's
Figure 9. FTIR-ATR spectra of diﬀerent standards formulated with APP (a), dechlorane (b) or TBBPA (c) – blue frame for FR characteristic peaks seen within polymer references
spectrum is heavily distorted. Its initial baseline (shifted here for readability) varies between 0.5 and 0.6 A.U. of absorbance for about 0.1 to 0.2 U.A. for intrinsic peak heights. Peaks also display defaults at their base, reminiscent of the≈20 wt% carbon black loaded PP and ABS ofFig. 6. High carbon black loading is coherent with the elasto-meric nature of this component. Identiﬁcation is here challenged, especially as this study focused on thermoplastics. The two peaks be-tween 2920 and 2850 cm−1could hint for an important ethylene base. Peaks roughly at 1000 and 800 cm−1could correspond to vinylic C-H deformation but do not match to PB (910 and 965 cm−1). Polyisoprene is a possible candidate.
The second sample (n°2.8) consists of a green bulk tinted poly-ethylene, identiﬁed by its simple spectrum, coated with a PVC sheet, white on one side, lighter green on the other side as seen on the picture. PVC is identiﬁed thanks to the 610 and 700 cm−1peaks. A plasticizer
and/or thermal additive presence is shown through the 1730 cm−1 peak. The last sample, n°4.19 results of the welding of two transparent sheets which could be identiﬁed as PC and PMMA thanks to carbonyl peak, respectively 1770 and 1720 cm−1 and characteristic C-O stretching patterns between 1300 and 1000 cm−1. Interestingly en-ough, in the welding zone, an intermediate spectrum can be obtained, with the peaks of both polymers, especially highlighted for the dual carbonyl peaks.
Several samples were categorized as“shiny grey HIPS”. As shown on
Fig. 11.b), they consist of dark grey bulk tinted HIPS with a shiny grey coating. Bulk is easily recognized as HIPS thanks to aromatic C-H bending at 695 and 750 cm−1(whereas it is 700 and 760 cm−1for ABS) (Signoret et al., 2019a). The shiny coating is rather thin and its spec-trum, even though distorted, is heavily reminiscent of PMMA, an acrylic polymer, notably with a C=O stretching at 1724 cm−1, rather speciﬁc pattern from 1480 to 1385 cm−1for C-H bending, culminating peak at 1143 cm−1for C-O stretching and a peak at 750 cm−1for C-H rocking (Szilasi et al., 2011). Acrylic paint is thus strongly suspected, as its main monomer is also methyl methacrylate.
If analyzed on “bulk” face, these samples would be identiﬁed as HIPS. On the other side, ATR spectra are heavily distorted and cannot be confused with PMMA. Similar eﬀects can be expected but must be
checked in MIR-HSI. It can be anticipated that this supposed paint would impact also other identiﬁcation technologies, as Raman spec-troscopy or frothﬂotation. Even if not found within the studied stock, metallized ABS is rather common, especially in ELV (End-of-Life Vehicles). These objects can be expected to be hard to identify as ABS. As the metal layer will surely be problematic during mechanical re-cycling, it can be positive to remain unidentiﬁed.
Other common “complex” objects were also found, as electrical cables, often combining mainly copper and PVC, screwed plastic parts, elastomer pads embedded in plastic, paper or plastic label. Metallic parts were found despite magnetic sorting probably because of their rather low concentration within plastic. All these objects could nega-tively impact recycling. First, they can disturb identiﬁcation. Secondly, they bring contaminants that can aﬀect processability and use proper-ties.
Nowadays, the industrial sorting of dark-colored End-of-Life plastics is an obstacle to their recycling, as one of the most spread sorting technologies, Near-Infrared Hyperspectral Imagery (NIR-HSI) is unable to perform this task. Mid-Infrared HSI (MIR-HSI) is one the potential answers to this issue.. Consequently, its laboratory equivalent, Fourier-Transform Infrared spectroscopy (FTIR), was here studied to evaluate the theoretical limits of its industrial equivalent. Possible dangers of decreased acquisition parameters were shown in theﬁrst part of this study. Resolution depreciation leads to convolution of close signals and acquisition time decrease alters Signal-to-Noise ratio (SNR). This is particularly detrimental to small and close peaks. Atmospheric species, namely carbon dioxide and water are visible in both MWIR (5000 to 2000 cm−1or 2 to 5 μm) and LWIR (1350 to 700 cm−1at max or 7.4 to 14.0 μm) but should not disturb polymer identiﬁcation as covered ranges or signal natures are diﬀerent.
Carbon black, which is prohibitive for polymer sorting in NIR-HSI, also impacts MIR spectroscopy. The main feature is an elevation of baseline. Identiﬁcation should however still be possible, especially with relatively low loadings associated to coloration and UV-protection (0.5
Figure 10. Spectra comparison of two waste samples respectively with virgin and 15 wt. % Dechlorane HIPS references and with virgin and 17 wt. % TBBPA ABS references– blue frame for RF characteristic peaks seen within polymer samples
to 2.0 wt. %). Higher loadings used for electrical conductivity or me-chanical reinforcement (mainly elastomers) strongly distort spectra and could negatively interfere with classiﬁcation algorithms.
Fillers, namely calcite, talc, kaolin and titanium dioxide, andﬂame retardants, namely APP, Dechlorane and TBBPA, were also described in MIR. Most of them display very few signals or none in MWIR. These signals are also often weak. Thus, they cannot be detected and will not disrupt polymer identiﬁcation in MWIR. Their signatures in LWIR are generally more intense and they cover large ranges, either by very broad signals or by very numerous peaks. Then, they can severely disrupt polymer identiﬁcation in LWIR. This disruption can be seen in several ways: polymer peaks are masked; additive peaks are recognized as belonging to another polymer; data amount and general signal ap-pearance are detrimental to algorithmic treatments. In this way, it is important to incorporate these pieces of information or, even better, altered spectra in a working database. In this purpose, these signals were here collected and described in this study.
Additives studied here were conditioned by what was rapidly available and what was identiﬁed within the studied plastic waste stock, mainly calcite and talc. Numerous other additives, especially ﬂame retardants or stabilizers, are to be found within plastic waste.
Thus, an exhaustive referencing in FTIR-ATR could be really interesting for both fast but rich laboratory analysis and possible impacts on in-dustrial sorting. After these signals are qualitatively identiﬁed, they could explain signiﬁcant diﬀerences found in a statistical study, espe-cially with the use of classiﬁcation algorithms. To consolidate these results, it would be then necessary, with the help of automatized methods, to extend the study to a larger waste stock, especially richer in ﬂame retarded samples.
This work was supported by BPI France via the FUI 20 (Fonds un-ique interministériel) grant.
CRediT author statement
Charles Signoret (PhD student): Writing - original draft, Conceptualization, Methodology, Investigation and rewriting revision manuscript.
All the authors: Visualization, Investigation and validation. Didier Perrin & Patrick Ienny: Supervision
Figure 11. Examples of complex real waste samples– a) several polymers within a sample - b) painted HIPS, spectra of both faces and comparison to PMMA and HIPS reference samples– blue frames for PMMA peaks, black for HIPS
The authors would like to express their appreciation toward
Benjamin Gallard, Robert Lorquet, Loïc Dumazert and Jean-Claude Roux from C2MA for technical support, respectively for polymer pro-cessing, spectroscopy experiments, thermal characterization and SEM/ EDX analysis. Marc-Adrien Tronche, PhD student at ENSCM, is also thanked for his advice about carbon black managing. Suez and Pellenc ST are gratefully acknowledged for partnership in this work. Finally, the authors are very thankful to Allize-Plasturgie for providing the numerous references of the Matériautech used in this work.
Appendix A. Examples TGA curves for concentration control of carbon black loaded ABS standard samples– under nitrogen until 670°C, oxygen beyond - magniﬁcation on gas switch zone
Appendix B. MIR spectra of ABS at diﬀerent carbon black loadings between 0.05 up to 4.5 w% - 5 spectra by sample, no normalization or numerical oﬀset – magniﬁcation on 2100-2000 cm-1 for low loadings – pictures of corresponding samples
Didier Perrin: Editing, Data curation, Reviewing. Declaration of Competing Interest
The authors declare that they have no known competing ﬁnancial interests or personal relationships that could have appeared to inﬂu-ence the work reported in this paper.
Appendix C. FTIR-ATR (MIR) spectra ofﬂame retardant powder references
Aldrian, A., Ledersteger, A., Pomberger, R., 2015. Monitoring of WEEE plastics in regards to brominatedﬂame retardants using handheld XRF. Waste Manag 36, 297–304.
Allen, N.S., Edge, M., Corrales, T., Childs, A., Liauw, C.M., Catalina, F., Peinado, C., Minihan, A., Aldcroft, D., 1998. Ageing and stabilisation ofﬁlled polymers: an overview. Polym. Degrad. Stab. 61, 183–199. https://doi.org/10.1016/S0141-3910(97)00114-6.
Ashkiki, A.R., Felske, C., McCartney, D., 2019. Impacts of seasonal variation and oper-ating parameters on double-stage trommel performance. Waste Manag 86, 36–48.
Bae, J.-S., Oh, S.-K., Pedrycz, W., Fu, Z., 2019. Design of fuzzy radial basis function neural network classiﬁer based on information data preprocessing for recycling black plastic wastes: comparative studies of ATR FT-IR and Raman spectroscopy. Appl. Intell. 49, 929–949.https://doi.org/10.1007/s10489-018-1300-5.
Barbier, S., Perrier, S., Freyermuth, P., Perrin, D., Gallard, B., Gilon, N., 2013. Plastic identiﬁcation based on molecular and elemental information from laser induced breakdown spectra: a comparison of plasma conditions in view of eﬃcient sorting. Spectrochim. Acta - Part B At. Spectrosc. 88, 167–173.https://doi.org/10.1016/j.sab. 2013.06.007.
Becker, W., Sachsenheimer, K., Klemenz, M., 2017. Detection of black plastics in the middle infrared spectrum (MIR) using photon up-conversion technique for polymer recycling purposes. Polymers (Basel) 9, 435.https://doi.org/10.3390/
Beigbeder, J., Perrin, D., Mascaro, J.-F., Lopez-Cuesta, J.-M., 2013. Study of the physico-chemical properties of recycled polymers from waste electrical and electronic equipment (WEEE) sorted by high resolution near infrared devices. Resour. Conserv. Recycl. 78, 105–114.https://doi.org/10.1016/j.resconrec.2013.07.006.
Bokobza, L., Bruneel, J.L., Couzi, M., 2013. Raman spectroscopic investigation of carbon-based materials and their composites. Comparison between carbon nanotubes and
carbon black. Chem. Phys. Lett. 590, 153–159.https://doi.org/10.1016/j.cplett. 2013.10.071.
Delva, L., Hubo, S., Cardon, L., Ragaert, K., 2018. On the role ofﬂame retardants in mechanical recycling of solid plastic waste. Waste Manag 82, 198–206.https://doi. org/10.1016/j.wasman.2018.10.030.
Fletcher, W.H., Rayside, J.S., 1974. High resolution vibrational Raman spectrum of oxygen. J. Raman Spectrosc. 2, 3–14.https://doi.org/10.1002/jrs.1250020102. Florestan, J., Lachambre, A., Mermilliod, N., Boulou, J.C., Marﬁsi, C., 1994. Recycling of
plastics: automatic identiﬁcation of polymers by spectroscopic methods. Resour. Conserv. Recycl. 10, 67–74.https://doi.org/10.1016/0921-3449(94)90039-6. Gallen, C., Banks, A., Brandsma, S., Baduel, C., Thai, P., Eaglesham, G., Heﬀernan, A.,
Leonards, P., Bainton, P., Mueller, J.F., 2014. Towards development of a rapid and eﬀective non-destructive testing strategy to identify brominated ﬂame retardants in the plastics of consumer products. Sci. Total Environ. 491–492, 255–265.https://doi. org/10.1016/j.scitotenv.2014.01.074.
Gent, M.R., Menendez, M., Toraño, J., Diego, I., 2009. Recycling of plastic waste by density separation: prospects for optimization. Waste Manag. Res. 27, 175–187.
Grause, G., Fonseca, J.D., Tanaka, H., Bhaskar, T., Kameda, T., Yoshioka, T., 2015. A novel process for the removal of bromine from styrene polymers containing bromi-natedﬂame retardant. Polym. Degrad. Stab. 112, 86–93.https://doi.org/10.1016/j. polymdegradstab.2014.12.017.
Grégoire, S., Boudinet, M., Pelascini, F., Surma, F., Detalle, V., Holl, Y., 2011. Laser-induced breakdown spectroscopy for polymer identiﬁcation. Anal. Bioanal. Chem. 400, 3331–3340.https://doi.org/10.1007/s00216-011-4898-2.
Gundupalli, S.P., Hait, S., Thakur, A., 2017. A review on automated sorting of source-separated municipal solid waste for recycling. Waste Manag 60, 56–74.https://doi. org/10.1016/j.wasman.2016.09.015.
Guzzonato, A., Mehlmann, H., Krumwiede, D., Harrad, S., 2016a. A novel method for quantiﬁcation of decabromodiphenyl ether in plastics without sample preparation using direct insertion probe– magnetic sector high resolution mass spectrometry. Anal. Methods 8, 5487–5494.https://doi.org/10.1039/C6AY00460A.